Size-controllable synthesis of ultrasmall diamonds from ... · PDF file Letter to the editor...
Embed Size (px)
Transcript of Size-controllable synthesis of ultrasmall diamonds from ... · PDF file Letter to the editor...
lable at ScienceDirect
Carbon 150 (2019) 436e438
Contents lists avai
journal homepage: www.elsevier .com/locate /carbon
Letter to the editor
Size-controllable synthesis of ultrasmall diamonds from halogenated adamantanes at high static pressure
https://doi.org/10.1016/j.carbon.2019.05.047 0008-6223/© 2019 Elsevier Ltd. All rights reserved.
a b s t r a c t
We report on the use of dibromoadamantane C10H14Br2 as a promising precursor for the mass synthesis of ultrasmall diamonds at an industrially accessible pressure of 8 GPa. Under pressure, the formation of nanodiamonds upon decomposition of C10H14Br2 starts at the record low temperature of 1000 К. As a result of the decomposition, effective nucleation of diamonds and their slow growth at temperatures up to 2000 K provide favorable conditions for the size-controlled synthesis of nanodiamonds by changing the synthesis temperature. We show that chloroadamantane, C10H15Cl, is also a good candidate for producing nanodiamonds.
© 2019 Elsevier Ltd. All rights reserved.
Great attention to the synthesis of diamonds from hydrocarbons at high pressures arises in connectionwith the possibility of obtain- ing diamond nanocrystals, doped with electrically and optically active impurities for nanotechnology applications [1,2]. It is assumed that in comparison with the diamond production under metastable (CVD) or highly non-equilibrium conditions (explosive technologies), the synthesis under high static pressures (HPHT) can provide the diamond formation with the highest structure perfection. Reduction of the potential barrier for the formation of diamonds from hydrocarbons in comparison with that of the direct graphite-to-diamond transition, allows obtaining diamonds at pressures of 8e9 GPa. However, so far well controllable mass syn- thesis of nanodiamonds at high static pressures has been carried out only in case of the highly boron-doped diamond; 9-Borabicy- clo[3.3.1]nonane dimer, C16H30B2, was used as a precursor for the production . Mass synthesis of pure nanodiamonds can be car- ried out from adamantane at 8e9 GPa, but in a very narrow temper- ature range of 1500e1600 K , which makes it impossible to control the process.
In this paper, we show that halogen derivatives of adamantane: C10H14Br2 (99% purity, Aldrich) and C10H15Cl (98% purity, Aldrich) are excellent precursors for mass synthesis of nanodiamonds at an industrially accessible pressure of 8 GPa. Possibility of the syn- thesis of ultrasmall diamonds with controllable crystal size is for the first time demonstrated on the example of C10H14Br2.
The samples were obtained in a high-pressure chamber of the toroid type at a pressure of 8 GPa. Compressed tablet of the initial material 4 mm in diameter and 4 mm in height was loaded into a graphite crucible-heater and a containermade of lithographic stone (CaCO3). The temperature was controlled by thermocouples, the junctions of which were placed on the outer side of the heater. The characteristic duration of the synthesis did not exceed 2 min. Diffraction patterns were obtained in the transmission
configuration using Mylar film as the sample holder. Micro- Raman measurements were performed at room temperature using 488 nm line of Ar þ ion laser for excitation. To avoid overheating, the laser power was kept at a minimum (~0.2 mW at the sample) and the 10� objective was used for laser focusing.
Decomposition of dibromoadamantane, detected by the mass loss (about 10%), starts at a temperature of 900 K; most of the ma- terial is retained in the original crystal structure (Fig. 1). At further increase of temperature, the samples lose 50e60% of the mass, forming an easily fragmented transparent glassy substance (about 40e50 mg in mass) with diamond peaks in x-ray diffraction pat- terns. As the synthesis temperature rises, diffraction peaks of dia- mond become narrower, indicating an increase of size of the diamond crystals. Relative changes in the crystal sizes were traced with use of the Williamson-Hall (for samples obtained at 1400e2000 K) and Scherrer (for the 111 x-ray diffraction peak) methods for calculation of crystallite sizes. Bothmethods gave close values probably due to relatively small inhomogeneous strains in synthesized nanodiamonds. The dimensionless shape factor was taken equal to unity in the calculations; change in the shape of nanocrystals was not taken into account. According to the calcula- tions, the average crystallite size monotonically increases from 1.5 nm to 46 nm with an increase in the synthesis temperature to 2000 K.
Direct measurements of nanocrystal sizes in the TEM images (Fig. 2) give values, well correlated with the calculated ones. The shape of diamond nanocrystals evolves from sphere-like to clearly facetted by the 111 faces with increasing synthesis temperature, which reflects the tendency to acquire an equilibrium shape depending on the ratio of surface and volume energies of crystals growing under certain conditions. Slightly elongated or flattened crystals, detected in samples (see Fig. 2a and b), were probably formed due to nonuniform temperature field in the reaction
http://crossmark.crossref.org/dialog/?doi=10.1016/j.carbon.2019.05.047&domain=pdf www.sciencedirect.com/science/journal/00086223 www.elsevier.com/locate/carbon https://doi.org/10.1016/j.carbon.2019.05.047 https://doi.org/10.1016/j.carbon.2019.05.047 https://doi.org/10.1016/j.carbon.2019.05.047
Fig. 1. Evolution of the x-ray diffraction patterns of samples and the average size of nanodiamonds (shown in the figure) obtained from 1,3-Dibromoadamantane with increasing synthesis temperature at a pressure of 8 GPa. As an example, the diffraction pattern of the sample synthesized at 1570 K from C10H15Cl is shown at the top of the figure. At small diffraction angles there are peaks originated from the Mylar sample holder (at 18 and 32�) and accidentally caught in the sample pieces of graphite heater (line 002 of graphite at 26�). D e diamond. (A colour version of this figure can be viewed online.)
Fig. 2. TEM images of nanodiamonds obtained at (a) 1600 K (insert shows diffraction pattern taken from an area of 500 nm in diameter on the sample, (b) 1400 K (insert demonstrates diffraction pattern taken from an area of 500 nm in diameter on the sample and (c) 1100 K (inserts show a diamond crystal with fine resolution and
Letter to the editor / Carbon 150 (2019) 436e438 437
volume. The data on Raman spectroscopy investigation of diamond samples are presented in Fig. 3. Apart from the diamond Raman line, the following features are detected in the spectra: lines at 1140 and 1450 cm-1 assigned to the trans-polyacetylene fragments, broad bands of the disordered sp2 carbon at 1350 and 1590-1620 cm-1 , and the line at 1340 cm-1.The intensities of all non- diamond Raman lines decrease with the increase of synthesis tem- perature and size of the synthesized nanodiamonds, indicating their association with the growth medium and surface states of nanodiamonds. In the sample obtained at 1000 K, the diamond Raman line is not detected. The high scattering cross-section of disordered sp2 carbon obviously shades the presence of the 1e2 nm diamonds in the sample. Systematic broadening and shift of the diamond Raman line from 1332 to 1324 cm-1 were detected for nanodiamonds with a decrease in the average crystal size pre- sumably due to the phonon confinement effect .
An interesting feature of the dibromoadamantane carbonization at 8 GPa is the absence of the stage of graphite formation, charac- teristic of pure hydrocarbons . It is known that bromine, like
diffraction pattern from the displayed diamonds). (A colour version of this figure can be viewed online.)
Fig. 3. Normalized Raman spectra of pristine C10H14Br2 (300 K) and nanodiamonds of various sizes. As an example, the Raman spectrum of the sample synthesized at 1570 K from C10H15Cl is shown at the top of the figure. The spectra are shifted vertically for clarity. (A colour version of this figure can be viewed online.)
Letter to the editor / Carbon 150 (2019) 436e438438
other halogens, actively reacts with unsaturated hydrocarbons and practically does not interact with saturated ones in the absence of catalysts or special conditions. For this reason, the bromination re- action is commonly used as a test to distinguish between saturated and unsaturated hydrocarbons. It can be assumed that during the decomposition of dibromoadamantane, bromine inhibits the for- mation of graphite with unsaturated bonds and stabilizes carbon clusters with sp3 hybridized carbon, giving rise to diamond nucle- ation and growth. At the same time, adsorption of bromine at the diamond surface is the most probable reason for very slow growth (recrystallization) of diamond crystals even at temperatures of 2000 K. If it is the case, the crystal growth is to a great extent
controlled by chemical reaction at the crystal surface. The appearance of the 1340 cm-1 line in the Raman spectra and
the absence of strong broad-band fluorescence, characteristic of nanodiamonds produced from pure adamantane , may be con- nected with the adsorbed bromine.
In a few of experiments, we have found that thermobaric treat- ment of C10H15Cl also gives the same results as processing C10H14Br2 in similar conditions (see Figs. 1 and 3).
The results obtained suggest that the cage molecule structure and specific bromine chemistry ensures the effective nucleation of diamonds and their slow growth in the CeHeBr system at tem- peratures up to 2000 K, providing favorable conditions for the controllable synthesis of nanodiamonds. We have shown that chlo- rinated adamantane is another good prec